Sabarmati River Front Development Corporation Limited Page 11 Specification for Hot Dip Zinc Galvanization of Steel (Rolled & Fabricated) 1.1 ScopeThis specification covers the general requirements of hot dip galvanizing for fabricated M.S. sections-plates, foundation bolts including cleaning of any paint, grease, rust, scale, acid or alkali or such otherforeign matters. 1.2 Applicable CodesThe following Indian Standard Codes, unless otherwise specified herein, shall be applicable.(i) IS: 4759-1979: Specification for Hot Dip Zinc Coatings on Structural Steel and other allied Products.(ii) IS: 209-1979: Specification for zinc.(iii) IS: 2629-1966: Recommended Practice for Hot Dip Galvanizing of Iron and Steel.(iv) IS: 6158-1971: Recommended Practice for Safe-guarding against Embrittlement of Hot Dip Galvanized Iron & Steel Product.(v) IS: 2633-1972: Method of Testing Uniformity of Coating on Zinc Coated Articles.(vi) IS: 6745-1972: Method for Determination of weight of Zinc Coating on Zinc coated iron and steel articles (with amendment No. 1).(vii) ASTM A-123: Spec. for Zinc (Hot Galvanized) Coatings on (1978) Products Fabricated from Rolled, Pressed and Forged Steel Shapes, Plates, Bars and Strips. 1.3 General Requirements1.3.1 QUALITY OF ZINC: Zinc conforming to at least grade Zn 99.95 specified in IS: 209-1979 shall be used for the purpose of galvanizing.1.3.2 BASE METAL: The steels and castings shall be in accordance with clause 2 of IS: 6158-1971. Where steel is supplied by the fabricator, it is the responsibility of the fabricator to select suitable steel which will withstand normal galvanizing operation without embrittlement. The edges of tightly contacting surfaces should be completely sealed by welding. The residue of coated electrodes should be removed, prior to pickling, by brushing, chipping or sand blasting. 1.3.3 SURFACE PREPARATION: Surface shall be cleaned and prepared as per clause 4 of IS: 2629- 1966. Malleable iron castings shall be shot and grit blasted before galvanizing. 1.3.4 GALVANISING: The members shall be galvanized in accordance with the practice contained in the IS: 2629-1966 unless otherwise specified in the succeeding paragraphs.
Sabarmati River Front Development Corporation Limited Page 2 1.4 Coating Requirements1.4.1 MASS OF ZINC COATING: Minimum average mass of zinc coating on different kinds of articles shall be as under: a) Fabricated steel Thickness less than 2 mm but not less than 1.2 mm 340 gms/sq.m Thickness 2 mm and above 750 gms/sq.m b) Fasteners Up to nominal size M10 270 gms/sq.m Over M10 300 gms/sq.m 2 Note: Articles galvanized with 1000 g/m zinc coatings shall be identified by a band of green paint by the galvanizer.1.4.2 FREEDOM FROM DEFECTS: The zinc coatings shall be uniform, adherent, reasonably smooth and free from imperfections such as flux ash and dross inclusions, bare patches, black spots, pimples, lumpiness and runs, rust stains, bulky white deposits and blisters, etc. These terms have been defined in IS: 2629-1966 (duly amended wherever necessary).1.4.3 STEEL EMBRITTLEMENT: The design of the product and the selection of steel, wherever steel is to be supplied by fabricator, for its suitability to withstand normal galvanizing operations without embrittlement or the method of fabrication shall be the responsibility of the fabricator. Recommended precautions to properly design, fabricate and prepare the material for galvanizing to prevent embrittlement shall be as per IS: 6158-1971. 1.5 Tests1.5.1 TYPE TESTS (a) Visual Inspection (b) Adhesion of coating (c) Uniformity of coating (d) Mass of zinc coating Each test shall be conducted on three samples.1.5.2 ACCEPTANCE TESTS (a) Visual Inspection (b) Adhesion of coating
Sabarmati River Front Development Corporation Limited Page 3 (c) Uniformity of coating (d) Mass of zinc coating1.5.3 ROUTINE TESTS (a) Visual Inspection 1.6 Scale of Sampling and criteria for conformity1.6.1 LOT: All the material of the same type in a coating bath whose characteristics are intended to be uniform shall be grouped together to constitute a lot. A lot shall not consist of more than one shift’s production or 100 nos. whichever is lower. Sample shall be taken from each bath and tested for conformity of coating. Where the galvanizing is done without the presence of Purchaser, the manufacturer may prepare lots consisting of the articles of the same type and material and galvanized in the same bath. If there are more than one bath, separate lots shall be prepared for each bath.1.6.2 SCALE OF SAMPLING: Samples in accordance with TABLE 1 shall be taken, at random, from each lot for tests. TABLE 1: Scale of Sampling Lot size Sample Permissible no. of size defective units Up to 25 3 0 26-50 5 0 51-100 8 0 101 and above 13 11.6.3 For materials of inconvenient lengths and from which it is not possible to cut a specimen for coating characteristic tests, two test pieces of same cross section and not less than 90 cms length shall be galvanized in the same bath.1.6.4 The samples selected in accordance with Table 1 above shall be subjected to the visual inspection. If any sample fails to conform to the requirement, the lot shall be rejected. The galvaniser, however, may segregate the good pieces of the lot and submit them once again for inspection.
Sabarmati River Front Development Corporation Limited Page 41.6.5 If the lot inspected for visual inspection, passes the test, 3 samples for coating characteristics shall be taken from the samples, which were subjected to the visual tests.1.6.6 Each of the 3 samples will be subjected to test for adhesion, uniformity, mass of zinc coating. Should any sample fail in any test, six more samples shall be taken from the lot and all the 3 tests repeated. Should any sample fail in the retest, the lot shall be rejected. If it is not possible to take six samples for the test, the lot shall be rejected.1.6.7 The material in a lot which has been rejected may be stripped and re-galvanized and submitted for inspection and tests. 1.7 TEST METHODS1.7.1 VISUAL INSPECTION: The material shall be inspected visually to observe that it is smooth, reasonably bright, continuous and free from such imperfections as flux/ash/dross inclusions, bare patches, black spots, pimples, lumpiness runs, rust stains, bulky white deposits and blisters. The stains of flux, usually white in colour, shall not be regarded as flux intrusions.1.7.2 ADHESION OF GALVANISED COATING:220.127.116.11 Coating shall withstand the knife tests as prescribed in IS: 2629-1966. When cut or pried into, such as with a stout knife applied with considerable pressure, in a manner tending to remove a portion of the coating, it shall only be possible to remove small particles of the coating; and it shall not be possible to peel any portion of the coating so as to expose iron or steel underneath.18.104.22.168 On articles fabricated from angles, channels, beams and rolled sections of 8 mm or more thickness, the adhesion may, alternatively, be tested by pivoted hammer tests as per IS : 2629- 1966. This test is not suitable for curved and round surfaces.1.7.3 UNIFORMITY OF GALVANISED COATING:22.214.171.124 On small articles, which can be conveniently handled the uniformity of the coating shall be determined by Preece Test in accordance with IS: 2633-1966 by dipping the whole article in the copper sulphate solution. For sheets, strips and other fabricated articles a 10 cm x 10 cm specimen may be cut for tests. For tubes, 100 mm long piece shall be cut from each end of the product, after discarding 300 mm length from the end. The article shall withstand 5 dips of one minute each.126.96.36.199 For long articles, measurement of coating thickness at a number of places by magnetic method shall be taken as a uniformity test. Note: The Preece Test is primarily meant for articles where surface is mechanically scrapped or wiped after dip in the galvanizing baths etc1.7.4 MASS OF GALVANISED COATING:
Sabarmati River Front Development Corporation Limited Page 188.8.131.52 The average mass of galvanized coating shall be determined by any one of the following methods as agreed between the purchaser and the galvaniser before the tests.184.108.40.206 Mass before and after galvanizing: The mass of coating may be determined by weighing the article before and after galvanizing, subtracting the first mass from the second and dividing the result by the coated surface area. The first mass shall be determined after pickling, rinsing and drying; and the second after cooling to the ambient temperature.220.127.116.11 Stripping method: In case of materials galvanized without purchasers’ inspection, average mass of coating shall be determined by stripping the entire article in accordance with IS: 6745-1972. If the surface area of the entire article cannot be measured easily or if the article is inconveniently large, a specimen of 100 sq. cm. area may be cut from each of the three samples and stripped. 1.8 Magnetic thickness gauge method:1.8.1 For large products such as poles, towers, structural shapes and castings the average weight of the coating shall be determined by a magnetic thickness gauge.1.8.2 Before making the measurement the gauge shall be calibrated by measuring the thickness of zinc coating on a test panel and comparing the measured value with the value obtained by stripping method on the same piece. For castings etc. at least 5 readings may be taken at convenient locations nearly in the centre. Thickness, in micro-meters, when multiplied by 7.047 would give the average mass of zinc 2 coating (g/m ). Three articles in each lot of up to 100 shall be tested in this manner.1.9 RECTIFICATION OF DAMAGE1.9.1 Normally all fabrication work in the case of galvanized articles shall be completed prior to galvanizing. If, for any reason, fabrication such as cutting, drilling or welding has to be undertaken after galvanizing, protection of metal exposed as a result of fabrication and rectification of damaged galvanized areas shall be done in accordance with either the following methods or any other method approved by the Purchaser.1.9.2 USE OF ZINC BASED SOLDERS: The surface to be protected, or the surface where galvanizing has been damaged, shall be cleaned and any oxides removed with a weak acid solution and a wire brush. The surface shall be thoroughly washed with water to make it free from any traces of acid. The cleaned area shall be heated with a welding torch and rubbed with white salammoniac. A piece of zinc stick or rod 5-10 mm diameter of high purity shall be melted on this area and spread out with a heated piece of salammoniac. The areas shall then be washed down by water and lightly wire brushed. The workmanship shall be such that the finished surface is smooth and non-porous.1.9.3 USE OF ZINC RICH PAINTS : The damaged surface after cleaning, as mentioned in para 7.2 shall be painted with two or more coats of zinc rich primer followed by a finishing coat of a zinc rich paint as per the painting schedule recommended by the manufacturers. It is to be ensured that the dry film thickness of zinc rich primer shall not be less than the average thickness of the
Sabarmati River Front Development Corporation Limited Page 6 galvanized coating. The complete painting system i.e. zinc rich primer with the finishing zinc rich paint for this purpose shall be produced from a source of repute and approved by the Purchaser. DEFECTS, THEIR CAUSES AND REMEDIAL MEASURES Ground for Defects Causes Recommended actions rejection Paint grease or oil residues Check cleaning practices Bare spots Scale or rust residues Check pickling practices Residual welding slag Blast-clean wells; avoid coated rods Breakdown of preflux Check preflux and drying coating conditions Yes, if bare spots are bigger than 8 Aluminum content of bath Regulate aluminum mm dia. or 8 mm too high additions diagonal. Rolling defects in basic Check steel supply steel Article in contact during Keep articles separated. galvanizing. Analysis or original surface Check steel supply. General condition of steel. roughness Over-pickling Reduce pickling use No inhibitor High galvanizing temperature or long Adjust galvanizing immersion time or both conditions. Pimples Entrapped dross particles Avoid agitation of dross No, unless dross layer; check carryover of contamination is pickle salt. heavy Withdrawal speed too high Remove work slowly Cold galvanizing bath. Increase temperature. Lumpiness Delayed run-off from Remove work slowly. and runs seams, joints, bolt holes, No. (uneven etc. drainage) Article in contact during withdrawal. Stale flux burnt on during Refresh or renew flux dipping. blanket. Flux inclusions Surface residues on steel. Check steel preparation. Yes. Flux picked up from top of Skim before withdrawal. bath. Ash burnt on during Skim bath before dipping. Yes, if in gross dipping. lumps.
Sabarmati River Front Development Corporation Limited Page 7 Ash inclusion Ash picked up from top of Skim before withdrawal. bath. Black spots Includes flux particles from Confine fluxing to top of Yes. flux ‘dusting’. bath. Dirt smuts, splash marks. Check storage conditions. No. Dull grey Steel composition (high sili- Check steel supply for No. coating (all con, phosphorous or composition order to adjust alloy, no free carbon) severe cold work. for galvanizing. zinc). Slow cooling after galvani- Avoid hot stacking quench. sing. Release of absorbed Avoid over pickling; use hydro-gen during inhibitor. solidification of coating. Weeping of acid etc. from Check product design and seams and folds. fabrication. Storage near rusty Rust stains Check storage condition. No. material. Bulky white Confinement of close Storage dry well-ventilated No. deposit (wet packed articles under damp conditions, separate storage stain, conditions. articles with spacer. white rust). Packing of articles while Dry before packing; include damp. desic cant. Expansion of entrapped Check steel quality hydrogen and moisture in flaws. Driving off of hydrogen Use shot blast instead of Blisters absorbed during pickling. pickle; check steel supply. Yes, if general. Improper malleabilising (for Check malleabilising malleable iron castings practice. only) Effect sometimes observed Use shot blast instead of Yes, if blistering is on quenched work notably pickle. Check malleabilising generally wide malleable castings. May be treatment. Should have no spread. caused by gas evolved combined carbon near Tiny blisters from the work resulting surface of casting. from absorbed hydrogen or break-down of combined carbon near surface.1.10 STRIPPING METHOD (Extracted from IS: 6745-1972)1.10.1 Cleaning of test piece : The test pieces shall be washed with solvent naptha, trichloro ethyleneor any other suitable organic solvent, then with alcohol and finally dried thoroughly.
Sabarmati River Front Development Corporation Limited Page 81.10.2 Stripping Solutions:Dissolve 20 g of antimony trioxide (Sb2O3) or 32 g of antimony trichloride (Sb Cl3) in 1000 ml ofconcentrated hydrochloric acid (specific gravity 1.1).Immediately before tests, prepare the stripping solution by adding 5 ml of the solution, 1 to 100 ml ofconcentrated hydrochloric acid (specific gravity 1.16). Mix well.1.10.3 Procedure – Weigh the cleaned test specimen whose mass is less than 200 g nearest to 0.01 g;for test piece whose mass is between 300 to 1000 g to the nearest 0.1 g; and for test specimen of over1000 g to the nearest 0.5 g. After weighing immerse each test piece singly in test solution and allow toremain there until the violent evolution of hydrogen and only a few bubbles are being evolved. Thisrequires about 15 to 30 seconds. 2The mass of zinc coating (in g/m ) of surface may be calculated as per the following formula: 6 M = M1 – M2 x 10 AWhere, 2M = mass of zinc coating, in g/m , of surface.M1 = original mass, in g, of test piece.M2 = mass in g, of 2stripped test piece, and A = coated area of the test piece, in mm .